#------------------------------------------------------------------------------
#$Date: 2016-02-16 03:10:39 +0200 (Tue, 16 Feb 2016) $
#$Revision: 176453 $
#$URL: svn://www.crystallography.net/cod/cif/7/10/09/7100956.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7100956
loop_
_publ_author_name
'Vladimir Fedorov'
'Svetlana Kozlova'
'Yu. V. Mironov'
'N. K. Moroz'
'D. Y. Naumov'
'A. Simon'
'S.F. Solodovnikov'
'S. S. Yarovoi'
_publ_section_title
;
Unexpected ligand substitutions in the cluster core
{Re6Se8}: synthesis and structure of the novel cluster compound
Cs11(H3O)[Re6Se4O4Cl6]3.4H2O
;
_journal_name_full               'Chemical Communications'
_journal_paper_doi               10.1039/b412850h
_journal_year                    2005
_chemical_formula_moiety         Cs11(H3O)[Re6Se4O4Cl6]3.4H2O
_chemical_formula_sum            'Cl18 Cs11 H11 O17 Re18 Se12'
_chemical_formula_weight         6682.32
_space_group_IT_number           148
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-R 3'
_symmetry_space_group_name_H-M   'R -3 :H'
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            6
_cell_length_a                   17.1360(3)
_cell_length_b                   17.1360(3)
_cell_length_c                   47.4916(14)
_cell_measurement_temperature    293(2)
_cell_volume                     12077.2(5)
_diffrn_ambient_temperature      293(2)
_exptl_crystal_density_diffrn    5.513
_cod_original_sg_symbol_H-M      'R -3'
_cod_original_formula_sum        'H11 Cl18 Cs11 O17 Re18 Se12'
_cod_database_code               7100956
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-x+2/3, -y+1/3, -z+1/3'
'y+2/3, -x+y+1/3, -z+1/3'
'x-y+2/3, x+1/3, -z+1/3'
'-x+1/3, -y+2/3, -z+2/3'
'y+1/3, -x+y+2/3, -z+2/3'
'x-y+1/3, x+2/3, -z+2/3'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Re1 Re 0.37097(4) -0.09173(4) 0.108950(13) 0.02289(16) Uani 1 1 d . . .
Re2 Re 0.37236(5) -0.07361(4) 0.057497(13) 0.02787(18) Uani 1 1 d . . .
Re3 Re 0.26528(4) -0.04921(4) 0.088605(13) 0.02848(18) Uani 1 1 d . . .
Re4 Re 0.39788(4) 0.06080(4) 0.118782(13) 0.02704(17) Uani 1 1 d . . .
Re5 Re 0.50435(4) 0.03655(4) 0.087629(13) 0.02839(18) Uani 1 1 d . . .
Re6 Re 0.40043(5) 0.08957(5) 0.064567(14) 0.03254(19) Uani 1 1 d . . .
Se1 Se 0.26676(13) -0.02810(13) 0.03607(4) 0.0425(5) Uani 1 1 d . . .
Se2 Se 0.29240(13) 0.10677(12) 0.09768(4) 0.0398(5) Uani 1 1 d . . .
Se3 Se 0.53189(12) 0.19326(11) 0.09657(4) 0.0383(4) Uani 1 1 d . . .
Se4 Se 0.50676(13) 0.05823(12) 0.03525(4) 0.0411(5) Uani 1 1 d . . .
Cl1 Cl 0.3529(3) -0.2108(3) 0.13825(8) 0.0285(9) Uani 1 1 d . . .
Cl2 Cl 0.3541(3) -0.1876(3) 0.02401(9) 0.0465(12) Uani 1 1 d . . .
Cl3 Cl 0.1029(3) -0.1308(3) 0.09544(11) 0.0532(13) Uani 1 1 d . . .
Cl4 Cl 0.4144(3) 0.1219(3) 0.16570(9) 0.0441(11) Uani 1 1 d . . .
Cl5 Cl 0.6561(3) 0.0674(3) 0.09322(11) 0.0527(13) Uani 1 1 d . . .
Cl6 Cl 0.4220(4) 0.2093(3) 0.03312(11) 0.0573(14) Uani 1 1 d . . .
Cs1 Cs 0.3333 -0.3333 0.07792(4) 0.0372(5) Uani 1 3 d S . .
Cs2 Cs 0.37518(8) -0.07932(8) 0.19758(3) 0.0417(3) Uani 1 1 d . . .
Cs3 Cs 0.64820(9) 0.14862(9) 0.16323(3) 0.0641(4) Uani 1 1 d . . .
Cs4 Cs 0.6667 0.3333 0.03239(4) 0.0509(6) Uani 1 3 d S . .
Cs5 Cs 0.59204(10) -0.11372(10) 0.03614(3) 0.0662(4) Uani 1 1 d . . .
O1 O 0.2610(7) -0.1761(7) 0.0819(2) 0.027(2) Uani 1 1 d . . .
O2 O 0.2825(7) -0.0629(6) 0.1334(2) 0.034(3) Uani 1 1 d . . .
O3 O 0.4812(7) 0.0066(7) 0.1316(2) 0.033(3) Uani 1 1 d . . .
O4 O 0.4599(7) -0.1030(7) 0.0819(2) 0.033(3) Uani 1 1 d . . .
O1W O 0.7951(12) 0.0307(11) 0.0390(4) 0.100(6) Uani 1 1 d U . .
O2W O 0.0000 0.0000 0.0665(15) 0.117(10) Uani 0.50 3 d SPU . .
O3W O 0.704(3) 0.336(5) 0.1942(11) 0.055(16) Uani 0.25 1 d PU . .
O4W O 0.951(4) 0.073(3) 0.0008(11) 0.055(14) Uani 0.25 1 d PU . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Re1 O4 2.076(11) . ?
Re1 O3 2.092(11) . ?
Re1 O1 2.136(10) . ?
Re1 O2 2.155(12) . ?
Re1 Cl1 2.359(4) . ?
Re1 Re4 2.4612(9) . ?
Re1 Re5 2.4612(9) . ?
Re1 Re2 2.4619(8) . ?
Re1 Re3 2.4625(9) . ?
Re1 Cs2 4.1241(13) 15_445 ?
Re1 Cs1 4.1302(9) . ?
Re1 Cs2 4.1824(13) 14 ?
Re2 O4 2.146(11) . ?
Re2 O1 2.173(10) . ?
Re2 Cl2 2.415(4) . ?
Re2 Se4 2.5143(18) . ?
Re2 Se1 2.5159(19) . ?
Re2 Re5 2.5412(9) . ?
Re2 Re3 2.5478(9) . ?
Re2 Re6 2.6113(9) . ?
Re2 Cs5 4.2671(16) 2_545 ?
Re2 Cs1 4.2684(8) . ?
Re2 Cs5 4.2731(16) . ?
Re3 O1 2.161(10) . ?
Re3 O2 2.179(10) . ?
Re3 Cl3 2.431(5) . ?
Re3 Se2 2.5108(18) . ?
Re3 Se1 2.5194(19) . ?
Re3 Re4 2.5470(9) . ?
Re3 Re6 2.6105(9) . ?
Re3 Cs2 4.2539(13) 15_445 ?
Re3 Cs3 4.3626(16) 15_445 ?
Re3 Cs5 4.4360(16) 2_545 ?
Re4 O3 2.144(10) . ?
Re4 O2 2.167(10) . ?
Re4 Cl4 2.418(4) . ?
Re4 Se2 2.5132(19) . ?
Re4 Se3 2.5151(18) . ?
Re4 Re5 2.5394(9) . ?
Re4 Re6 2.6178(9) . ?
Re4 Cs3 4.2602(16) 15_445 ?
Re4 Cs3 4.3204(15) . ?
Re4 Cs2 4.3575(13) . ?
Re5 O4 2.134(11) . ?
Re5 O3 2.139(10) . ?
Re5 Cl5 2.395(5) . ?
Re5 Se4 2.5125(18) . ?
Re5 Se3 2.5193(18) . ?
Re5 Re6 2.6105(9) . ?
Re5 Cs3 4.2335(16) . ?
Re5 Cs2 4.2888(13) 14 ?
Re5 Cs5 4.3287(16) . ?
Re6 Cl6 2.413(5) . ?
Re6 Se4 2.555(2) . ?
Re6 Se1 2.555(2) . ?
Re6 Se2 2.5557(19) . ?
Re6 Se3 2.5574(19) . ?
Se1 Cs5 3.964(2) 2_545 ?
Se1 Cs5 4.200(2) 10_655 ?
Se2 Cs3 4.058(2) 15_445 ?
Se3 Cs4 3.853(2) . ?
Se3 Cs3 4.013(2) . ?
Se4 Cs5 3.889(2) . ?
Se4 Cs4 4.1027(18) . ?
Se4 Cs5 4.108(2) 10_655 ?
Cl1 Cs1 3.468(4) . ?
Cl1 Cs2 3.493(4) 15_445 ?
Cl1 Cs2 3.508(4) . ?
Cl1 Cs2 3.514(4) 14 ?
Cl2 Cs1 3.468(5) . ?
Cl2 Cs4 3.556(5) 10_655 ?
Cl2 Cs5 3.620(5) 2_545 ?
Cl2 Cs5 3.661(5) . ?
Cl3 Cs2 3.493(5) 15_445 ?
Cl3 Cs3 3.920(6) 15_445 ?
Cl3 Cs5 4.040(6) 2_545 ?
Cl4 Cs3 3.449(5) 3_665 ?
Cl4 Cs2 3.510(5) . ?
Cl4 Cs3 3.699(5) 15_445 ?
Cl4 Cs3 3.801(5) . ?
Cl5 Cs2 3.479(5) 14 ?
Cl5 Cs3 3.633(6) . ?
Cl5 Cs5 3.844(6) . ?
Cl6 Cs5 3.629(6) 10_655 ?
Cl6 Cs4 3.631(5) . ?
Cs1 O4 3.428(11) 2_545 ?
Cs1 O4 3.428(11) . ?
Cs1 O4 3.428(11) 3_655 ?
Cs1 Cl2 3.468(5) 2_545 ?
Cs1 Cl2 3.468(5) 3_655 ?
Cs1 Cl1 3.468(4) 2_545 ?
Cs1 Cl1 3.468(4) 3_655 ?
Cs1 O1 3.490(10) . ?
Cs1 O1 3.490(9) 2_545 ?
Cs1 O1 3.490(9) 3_655 ?
Cs2 O1 3.383(10) 14 ?
Cs2 O4 3.476(10) 15_445 ?
Cs2 Cl5 3.479(5) 15_445 ?
Cs2 O3 3.482(10) 15_445 ?
Cs2 O2 3.489(10) 14 ?
Cs2 Cl1 3.493(4) 14 ?
Cs2 Cl3 3.493(5) 14 ?
Cs2 O2 3.511(10) . ?
Cs2 Cl1 3.514(4) 15_445 ?
Cs2 O3 3.552(10) . ?
Cs3 O2 3.016(12) 14 ?
Cs3 O3W 3.05(6) 3_665 ?
Cs3 O3 3.067(11) . ?
Cs3 O3W 3.21(6) . ?
Cs3 Cl4 3.449(5) 2_655 ?
Cs3 Cl4 3.699(5) 14 ?
Cs3 Cl3 3.920(6) 14 ?
Cs3 Se2 4.058(2) 14 ?
Cs4 Cl2 3.556(5) 10_655 ?
Cs4 Cl2 3.556(5) 11_665 ?
Cs4 Cl2 3.556(5) 12 ?
Cs4 Cl6 3.631(5) 2_655 ?
Cs4 Cl6 3.631(5) 3_665 ?
Cs4 Se3 3.853(2) 2_655 ?
Cs4 Se3 3.853(2) 3_665 ?
Cs4 Se4 4.1027(18) 2_655 ?
Cs4 Se4 4.1027(18) 3_665 ?
Cs5 O1W 3.105(17) . ?
Cs5 O1 3.176(10) 3_655 ?
Cs5 O4 3.209(11) . ?
Cs5 Cl2 3.620(5) 3_655 ?
Cs5 Cl6 3.629(6) 10_655 ?
Cs5 Se1 3.964(2) 3_655 ?
Cs5 Cl3 4.040(6) 3_655 ?
Cs5 Se4 4.108(2) 10_655 ?
Cs5 Se1 4.200(2) 10_655 ?
O1 Cs5 3.176(10) 2_545 ?
O1 Cs2 3.383(10) 15_445 ?
O2 Cs3 3.016(12) 15_445 ?
O2 Cs2 3.489(10) 15_445 ?
O3 Cs2 3.481(10) 14 ?
O4 Cs2 3.476(10) 14 ?
O3W O3W 1.07(7) 3_665 ?
O3W O3W 1.07(7) 2_655 ?
O3W Cs3 3.05(6) 2_655 ?
